The Role of Titanium Atom as a Catalyst for the Dissociation of Hydrogen on a Mg(0001) Aijun Dua,b, Sean C. Smitha,b, X.D.Yaob,c and G.Q.Lub aCentre bARC for Computational Molecular Science, Chemistry Building, The University of Queensland, Qld 4072 Centre for Functional Nanomaterial, School of Engineering, The University of Queensland, Qld 4072 cSchool of Engineering, James Cook University, Townsville, Qld 4811 Results and Discussion (continued) Introduction Among the metal hydrides under study as possible hydrogen storage media, magnesium hydride is one of the most promising candidates for the automotive application due to its very high capacity in the stoichiometric limit (7.6 weight %) and low cost . Unfortunately, the application is primarily limited by the hydrogenation reaction temperature and slow kinetics. One of the possible reasons is that the hydrogen molecules do not readily dissociate on Mg surface . Computational Method Jellium model (LDA) Dissociation Barrier Reference 0.50 eV Ref.  Experimentally, many studies have been devoted to the catalytic effect on hydrogen adsorption of mixing transitional metals into Mg powder during ball milling [3-4]. The transitional metals have been considered to act as catalysts for accelerating hydrogen sorption, i.e. enhancing the breaking up of the molecular hydrogen into adsorbed atoms . However, the catalytic mechanism involved when using these additives is still not clearly established. DFT (LDA) PES 0.37 eV Ref.  DFT (PBE) and NEB 1.15 eV Ref.  DFT (LDA) and NEB 0.35 eV This work PAW (PBE) and NEB 1.05 eV This work We report H2 interactions with both pure and Ti-incorporated Mg(0001) surfaces were studied by ab initio DFT calculations and the Nudged Elastic Band (NEB) method. The dissociation barrier of H2 on a clean Mg(0001) surface was first calculated and compared with other existing theoretical studies. The energetic for dissociation of H2 on the Ti-incorporated Mg(0001) surface was then computed and the catalytic role of the transition metal was elaborated. Computational Methodology TABLE I Comparison of present calculations for the activation barrier of hydrogen dissociation on a Mg(0001) surface with previous theoretical studies. IS 0.0 -0.2 Relative Energy (eV) Theoretically, ab initio DFT calculations have shown considerable predictive power for catalysis and could proved much insight on designing alloy catalysts . There have been some theoretical calculations to study the role of transition metals in magnesium hydride, but they are mainly limited to bulk calculation by substituting one Mg atom with a Ti, Ni or Fe atom. Only very a few calculations on the dissociative chemisorption of H2 onto a pure magnesium surface has been performed to establish the energetically favored pathway and the activation barrier in this process . To further clarify the role of transition metal in relation to recent experimental findings, investigations on the dissociation of H2 on transition metal incorporated Mg surfaces are highly desirable. TS1 -0.4 -0.6 LS1 -0.8 FS -1.0 LS2 -1.2 -1.4 Ab initio PAW Method: The calculations were performed mainly using the plane-wave basis VASP code  implementing the generalized gradient approximation (GGA) of PBE exchange correlation functional . An all-electron description, the projector augmented wave method (PAW) , is used to describe the ectronic-ion-core interaction. Using the PAW method, the lattice constant of bulk Mg was calculated to be 3.191 Å, which was only 0.5% in error compared with the experimental value. The cutoff energy for plane waves is chosen up to 312.5 eV for a very accurate energy calculation. The pure and Ti-incorporated Mg(0001) surface were modeled by using a (2×2) and a (3×3) surface unit cell with 5 layers of Mg atoms, respectively. A (4×4×1) Monkhost-Pack grid and 3-kpoints were used in the Brillouin-zone sampling for each surface. The vacuum space was at least 15 Å, which was large enough to guarantee a sufficient separation between periodic images. Additionally, using the ESPRESSO/PWSCF code , we have carried out DFT calculations based on the plane wave pseudopotential approach with the Local Density Approximation (LDA) only for the purpose of comparison with other existing theoretical results. Nudged Elastic Band Method: To determine dissociation barriers and Minimum Energy Paths (MEP), the NEB method was used . This method involves optimizing a chain of images that connect the reactant and product state. Each image is only allowed to move into the direction perpendicular to the hyper-tangent. Hence the energy is minimized in all directions except for the direction of the reaction path. A damped molecular dynamics was used to relax ions until the force in each image are less than 0.02 eV/Å. 0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30 Image Number Index (a) (b) (d) (c) (e) (f) Results and Discussion 1.1 1.0 Relative Energy (eV) 0.9 0.8 0.7 (g) 0.6 (h) (i) 0.5 Figure 3 (a) The minimum-energy-pathway profile for the dissociation of a hydrogen molecule on a Ti-incorporated Mg(0001) surface. IS, LS1, TS1, LS2 and FS represent the initial state, first local minimum state, first transition state, second local minimum state and final state, respectively. The dissociation pathway for a hydrogen molecule on a Ti-incorporated Mg(0001) surface. (b) a side and (c) a top view of the initial state (IS). (d) A side view of the first local minimum state (LS1). (e) The same as (d) but a top view. (f) The first transition state (TS1). (g) The second local minimum state (LS2). (h) The second transition state (TS2). (i) The final state (FS). The black, grey and small white balls represent Mg, Ti and H atoms, respectively. 0.4 0.3 0.2 0.1 0.0 0 10 20 30 40 Image numbers (a) (b) Conclusions Dissociative chemisorption of molecular hydrogen on both pure and Ti-incorporated Mg(0001) surfaces have been studied utilizing ab initio DFT calculations and the NEB method. Our results for the dissociation of H2 on a Mg(0001) surface were in good agreement with existing published work. For the Ti-incorporated Mg(0001) surface, the activated barrier was much smaller (0.103 eV) due to the strong interaction between the molecular orbital of H2 with the metal d orbitals. This could explain the experimentally-observed improvement in absorption kinetics of H2 when transition metals have been introduced into the Mg materials. References  Schwarz, R.B MRS Bull. 1999, 24, 40. Aschlapbach, L.; Zuttel, A. Nature 2001, 414, 23.  Liang, G.; Huot, J.; Van Neste, A.; Schulz, R. J Alloys Compounds 1999, 292, 247. Zaluska, A.; Zaluski, L.; Strom-Olsen, J.O. Appl.Phys.A: Mater.Sci. Process. 2001, 72, 157. (c) (d)  Von Zeppelin, F.; Reule, H.; Hirscher, M. J Alloys Compounds 2002, 330-332, 723.  Bobet, J.L.; Chevalier, B.; Darriet, B. J Alloys Compounds 2002, 330, 738.  Hanada, N.; Ichikawa, T.; Fujii, H. J.Phys.Chem B 2005, 109, 7188.  Greeley, J.; Mavrikakis, M. Nature materials 2004, 3, 810. Vang, R.T.; Honkala, K.; Dahl, S.; Vestergaard, E.K.; Schnadt, J.; Egsgaard.E.; Clausen, B.S.; Norskov, J.K., Besenbacher, F. Nature materials 2005, 4, 160.  Norskov, J.K.; Houmoller, A. M. Phys.Rev.Lett. 1981, 46, 257; Bird, D.M.; Clarke, L.J.; Payne, M.C.; Stich, I. Chem.Phys.Lett. 1993, 212, 518; Vegge, T. Phys.Rev.B 2004, 70, 035412.  Kresse, G.; Furthmuller, J. Comput. Mater. Sci 1996, 6, 15. Kresse, G.; Furthmuller, J. Phys.Rev.B 1996, 54, 11169.  Perdew, J.P.; Burke, K.; Ernzerhof, M. Phys.Rev.Lett. 1996, 77, 3865.  Blochl, P.E. Phys.Rev.B 1994, 50, 17953. Kresse, G.; Joubert, D. Phys.Rev.B 1999, 59, 1758.  Baroni, S.; Dal Corso, A.; de Gironcoli, S.; Giannozzi, P. http://www.pwscf.org.  Henkelman, J.; Jónsson, H. J. Chem. Phys., 2000, 113, 9978. Henkelman, J.; Uberuaga, B.P. ; Jónsson, H. J. Chem. Phys., 2000, 113, 9901. (e) (f) Acknowledgements Figure 1 The energetically preferred pathway and corresponding energy profile for the dissociation of a hydrogen molecule on a Mg(0001) surface. (a) Mg(0001) surface. A and B represent a hcp and fcc site, respectively. (b) The MEP. (c) Top view of the initial state (IS). (d) The same as (c) but a side view. (e) Top view of the transition state (TS). (f) Top view of the final state (FS). The black and white balls represent Mg and H atoms, respectively. We acknowledge generous grants of high-performance computer time from both the Computational Molecular Science cluster computing facility at The University of Queensland and the Australian Partnership for Advanced Computing (APAC) National Facility. The authors also greatly appreciate the financial support by Australian Research Council through the ARC Center for Functional Nanomaterials.